CHAPTER 15Corrosion Protection of SteelStructuresIntroductionAs pointed out in Chapter 2, the responsibility of a professional structural engineerin the 21st century is not confined to the usual considerations of economy, safety,and aesthetics alone. The present-day design consideration include the long-termenvironmental impact and also the life-cycle cost. Hence more importance is givenin current design codes to the durability of structures. It has to be recognized thatthe neglect of durability considerations has resulted in the degradation of severaltypes of structures in almost all cities of India irrespective of whether they aremade of reinforced concrete, prestressed concrete, or structural steel. Manyengineers believe that structural steel alone is not durable because of the problemof corrosion. As discussed in Chapter 2, durability and corrosion are considered asa serviceability limit state criteria. In this chapter we will discuss some methodsthat are used to prevent corrosion. The choice of the method depends on the severityof environment, the importance of structure, and the cost involved (the initial andthe life-cycle cost). A durable steel structure may be defined as the one that performs satisfactorilythe intended function(s) in the working environment under the anticipated exposureconditions during its service life, without any deterioration of the cross-sectionalarea and loss of strength due to corrosion. Thus the material used, the detailing,fabrication, erection, and surface protection measures should all address thecorrosion reduction and durability requirements. Before discussing the variousmethods that are available to prevent corrosion, let us discuss the mechanism ofcorrosion.15.1 Corrosion of SteelIron is thermodynamically stable in its oxide form. Iron oxide is refined to obtainsteel, which is thermodynamically unstable. Its tendency to corrode, and therebyto return to the stable state, is a fault of nature which cannot be changed. Iron andsteel, the most commonly used metals, corrode in many media including most
15.2 Design of Steel Structuresoutdoor atmospheres. As discussed in Chapter 1, the final products of steel areproduced by rolling, drawing, or forging. During hot rolling and forging the steelsurface is oxidized by air and a scale is produced, called mill scale. In the air, thepresence of mill scale on steel may reduce the corrosion rate over comparativelyshort periods, but over longer periods the rate tends to rise. In water, severe pittingof steel may occur if large amounts of mill scale are present on the surface of steelsections. Corrosion processes are usuallyelectrochemical in nature, having theessential features of a battery shown inFig. 15.1, consisting of an anode and acathode immersed in a solution ofelectrolyte (ASMI 1987). As shown inthe figure, when two bodies of differentelectric potentials are connected Fig. 15.1 Corrosion mechanism in a batteryelectrically in the presence of anelectrolyte, the anodic body provides electrons to the cathode. In this process theanode gets destroyed. Steel covered with mill scale can suffer severe attacks at small interruptions inthe scale when exposed to humid atmosphere or water containing salt. The millscale acts as the cathode, and the exposed steel at the discontinuity acts as theanode. In the presence of water and oxygen, which act as the electrolyte, a miniaturebattery is formed on the surface. In this case, the attack is more severe since theanode is small compared to the cathode. The effect is concentrated at the smallanode and the attack can produce serious pitting at the breaks in the scale (Gaylordet al. 1992). Ferrous ions travel into the solution from the anodic areas(see Fig. 15.2). The electrons (shown as e in the figure) that are released from theanode, move to the cathode, combine with water and oxygen present in theatmosphere to form hydroxyl ions. The reactions that occur are the following. Fig. 15.2 Corrosion mechanism in steel membersAt the anode Fe = Fe++ + Ze (steel) (ferrous ions) (electrons)At the cathode O2 + 2H2O + 4e = 4(OH) (oxygen) (moisture) (electrons) (hydroxyl ions)
Corrosion Protection of Steel Structures 15.3The ferrous ions react with the hydroxyl ions: 2Fe++ + 4(OH) = 2Fe(OH)2 (ferrous ions) (hydroxyl ions) (ferrous hydroxide) The ferrous hydroxide then oxidizes to hydrated ferrous oxide (Fe2O3 H2O)otherwise known as rust (which is browny red in colour). Now, there will be adifference between the electrical potentials of the cathodic surface that is coveredby rust (oxide film) and the non-corroded surface and, hence, the non-corrodedanode will corrode, forming rust on its surface. This type of cyclic reactions willresult in the formation of numerous miniature batteries and subsequent corrosionof the entire surface. Pollutants in the air, e.g., sulphur dioxide from the industrialatmosphere and salt from the marine atmosphere, increase the electrical conductivityof water and accelerate the corrosion reaction. From the above description, it maybe clear that the elimination of water, oxygen, or the electrical conductivity reducesthe rate of corrosion (www.corrosion-doctors.org). Most of the corrosion-resistantsystems try to eliminate any one or all the three elements in order to containcorrosion. Rust builds up as a deposit on the surface and may eventually flake off. Thecoating of rust does not inhibit corrosion, except in special steels, and corrosionprogresses beneath the rust and forms conical pits, thus reducing the thickness ofthe metal. The conical pits can act as stress raisers, i.e., the location of high localstresses, and in places subject to cyclic loads (e.g., cranes and bridges) may becomethe initiating points of fatigue cracks or brittle fracture.15.1.1 Types of CorrosionThe types of corrosion encountered in structural steel elements may be classifiedinto the following: l Uniform corrosion l Pitting corrosion l Crevice corrosion l Galvanic corrosion l Fretting corrosion l Stress corrosion l Intergranular corrosion l Bacterial corrosion l Erosion corrosion l Corrosion fatigue l Hydrogen embrittlementWe will briefly discuss these types of corrosion in this section.Uniform corrosion Uniform corrosion is characterized by a corrosive attackproceeding evenly over the entire surface area or a large fraction of the total area.A general thinning of the section takes place until failure. On the basis of tonnagewasted, this is the most important form of corrosion. However, uniform corrosionis relatively easily measured and predicted, making disastrous failures relatively
15.4 Design of Steel Structuresrare. It is undesirable from an appearance standpoint and can be controlled by theuse of coatings, paints, or cathodic protection. The breakdown of protective coatingsystems on structures often leads to this form of corrosion. In some cases, uniformcorrosion can add colour and appeal to the surface (e.g., the patina created bynaturally tarnishing copper roofs and the rust hues produced on weathering steel).Pitting corrosion Pitting corrosion is a localized form of corrosion resulting incavities in the surface of steel. It is more dangerous than uniform corrosion since itis more difficult to detect, predict, and design against. Corrosion products (rust)often cover the pits. As already mentioned, in addition to the loss of thickness,corrosion pits act as stress risers and may initiate fatigue and stress corrosioncracking. One pit in a large system may be sufficient enough to produce a catastro-phic failure of the entire system. An example of such a failure was the failure of agasoline line running over a sewer line, which killed 215 people, in Guadalajaru,Mexico (www.corrosion-doctors.org). This form of corrosion can be avoided byeliminating the presence of water by proper detailing and allowing free flow of airto dry the surface.Crevice corrosion Crevice corrosion is a locali-zed form of corrosion, usually associated withstagnant water in crevices (shielded areas) suchas those formed under gaskets, washers, insulationmaterial, fastener heads (see Fig. 15.3), threads,lap joints, and clamps. The oxygen content ofthe trapped water in a crevice reduces (than that Fig. 15.3 Crevice corrosionof the water exposed to air) and hence thecrevice becomes anodic with respect to the surrounding metal. This initiatescorrosion inside the crevice. Proper detailing can eliminate this form of corrosion.Galvanic corrosion Galvanic corrosion (also called bimetallic corrosion ordissimilar metal corrosion or sometimes wrongly as electrolysis) refers to thecorrosion damage induced when two (or more) dissimilar metals (e.g., iron andaluminium) are coupled in a corrosive electrolyte. Luigi Galvani invented this typeof corrosion in the eighteenth century and this led to the invention of the battery byAllessandro Volta in 1800. Galvanic corrosion occurs because metals in generalcan be arranged in terms of their electric potential into a table called the galvanicseries. The farther the metal in the galvanic series, the greater will be the tendencyfor the less noble material to corrode. A good example is the corrosion of steelscrews in stainless steel members and steel bolts in aluminium members. Galvaniccorrosion is common and can be destructive (a notable example is the galvaniccorrosion of the Statue of Liberty, USA). Designing to avoid any contact betweendissimilar metals can solve problems due to this type of corrosion. It is interesting to note that Sir Humphrey Davy and Michael Faraday used theprinciple of galvanic corrosion in the early nineteenth century to develop cathodicprotection of metals such as zinc, magnesium, and aluminium (see Section 15.2.6).
Corrosion Protection of Steel Structures 15.5Fretting corrosion Fretting corrosion refers to the corrosion damage that occursat the interface of two highly loaded surfaces that are not designed to move (rub)against each other. The most common type of fretting is caused by vibration. Theprotective film on the metal surface is removed by the rubbing action and exposesthe bare metal surface to the corrosive action of the atmosphere. The exposed areabecomes active compared with the rest of the protected metal surface. This kind ofcorrosion is found in machinery, bolted assemblies, and ball or roller bearings.Stress corrosion Stress corrosion cracking is thecracking induced by the combined influence oftensile stress and a corrosive environment (seeFig. 15.4). The required tensile stresses may be inthe form of directly applied stresses or in the formof residual stresses. Residual stresses are introducedby cold deformation and forming, welding, heattreatment, machining, and grinding. Stress corrosioncracking is a catastrophic form of corrosion, as thedetection of such fine cracks is difficult to predict. Fig. 15.4 Stress corrosionA disastrous failure may occur unexpectedly, with crackingminimal overall material loss. Stress corrosion cracking may lead to failure depending on the crack size, stresslevel, and temperature (corresponding to the conditions of brittle fracture). A typicalexample of this type of failure was the failure of the Silver Bridge across the OhioRiver in USA in 1967, which resulted in the loss of 40 lives (Gaylord et al. 1992).This structure had eye bars with large pin connections, which were not accessiblefor inspection. A very small crack in one of the eye bars caused a fracture, resultingin the subsequent failure of other eye bars due to overload and subsequent completecollapse of the bridge.Intergranular corrosion The microstructure of metals and alloys is made up ofgrains, separated by grain boundaries. Intergranular corrosion is a localized attackalong the grain boundaries or immediately adjacent to grain boundaries. A classicexample is the sensitization of stainless steel or weld decay. Reheating a weldedcomponent during multi-pass welding is a common cause of this problem. Chloridestress corrosion is a type of intergranular corrosion and occurs in austenitic stainlesssteel under tensile stress in the presence of oxygen, chloride ions, and hightemperature. It starts with chromium carbide deposits along the grain boundarieswhich leave the metal open to corrosion. Maintaining a low chloride ion and oxygencontent in the environment and the use of low carbon steel control this form ofcorrosion. The failure of a suspended ceiling over a swimming pool in Ulster,Switzerland, in 1985, resulted from this type of corrosion. The chlorine in the airabove the pool produced corrosion of the stainless steel hangers supporting thesuspended ceiling (Gaylord et al. 1992).Bacterial corrosion Bacterial corrosion is due to the result of the microbiologicalactivity and occurs in metal in contact with water or soil. Such corrosion is mostcommon in pipelines, buried structures, and splash zones of offshore structures.
15.6 Design of Steel StructuresErosion corrosion Erosion corrosion is the acceleration in the rate of the corrosionattack in a metal due to the relative motion of a corrosive fluid and the metalsurface. The increasing turbulence caused by pitting in the internal surfaces of atube can result in rapidly increasing erosion rates and eventually to a leak. Erosioncorrosion can also be aggravated by faulty workmanshipburrs left at the cut tubeends cause turbulence in the water flow, resulting in erosion corrosion. A combi-nation of erosion and corrosion leads to high pitting rates.Corrosion fatigue Corrosion fatigue is the result of the combined action of analternating stress and a corrosive environment. The introduction of a corrosiveenvironment often reduces the normal fatigue limit of a ferrous alloy, thereby crea-ting a finite life regardless of the stress level. No metal is immune from somereduction in its resistance to cyclic stressing if the metal is in a corrosive environ-ment. The control of corrosion fatigue is accomplished by either lowering the cyclicstress or by corrosion-protection methods.Hydrogen embrittlement This type of deterioration involves the ingress of hydrogeninto a component, which reduces the ductility and load-bearing capacity of themetal, which causes cracking and catastrophic brittle failures at stresses well belowthe yield stresses. An example of hydrogen embrittlement is the cracking ofweldments or hardened steels when exposed to conditions which inject hydrogeninto the component. Hydrogen embrittlement does not affect all metallic materialsequally and is not a permanent condition. High-strength steels, titanium, andaluminium alloys are vulnerable to hydrogen embrittlement. Hydrogen embrittle-ment can be avoided by controlling the amount of the residual hydrogen in steeland restricting the amount of in situ hydrogen introduced during the service life ofthe structural part. Though hydrogen embrittlement is included in the discussionabout corrosion, it is not really a corrosion phenomenon.18.104.22.168 Loss due to corrosionUnless rust-preventing measures are taken, structures made of steel will graduallydeteriorate in strength and other properties and the service life of the structure willbe shortened. The result of the surveys conducted in selected countries on theannual loss due to corrosion (see Table 15.1) shows that the figures are staggering.Table 15.1 Survey of annual loss due to corrosion Country Survey year Loss amount % of GNP Japan 1974 2,550,930 million yen 1.8 USA 2001 276 billion US dollars 3.2 UK 1970 1,365 million pounds 3.5 West Germany 1968-69 19,000 million Deutche marks 3.5 Australia 1973 470 million Australian dollars 1.5Source: Steel today and tomorrow 1989
Corrosion Protection of Steel Structures 15.7However, with suitable corrosion-control methods, the rate of corrosion can bemade very slow or practically nil, giving steel structures a long lease of life. Table 15.2 shows the average annual loss in the thickness of untreated steel inthe temperate zone.Table 15.2 Corrosion due to environment Environment Average corrosion losses (mm/year) Rural and mountainous with clean air 0.010.03 Urban and moderately industrial 0.030.06 Sea side and industrial 0.060.12 Chemical/Industrial 0.120.3The relationship between the thickness of the rust layer and the loss in the thicknessof steel is given by (Matsushima 1997) trt = Hr Sr1trl/(100Hs) (15.1)where trt is the loss in the thickness of steel (mm), Hr is the apparent specific gravityof rust, Hs is the specific gravity of steel (7850 kg/m3), trl is the thickness of the rustlayer (mm), and Srl is the Fe content of the rust layer (%). It has to be borne in mind that the thickness of the rust layer will be substantiallygreater (about three to four times) than the thickness lost in the original steel.15.1.2 Rate of CorrosionThe rate of corrosion depends on the following parameters: l Type of metal alloy l Humidity (in humid areaswhere humidity is greater than 70%or where air is saturated with industrial effluents, the corrosion rate of low carbon steel is nearly 100 times as great as in the dry location) l Rainfall l Temperature variations l Atmospheric pollution l Condensation of moisture l Chemical fumes l pH value l Oxygen content l Dissolved gasses (in the case of structures submerged in water or soil) As already discussed, the local corrosion rates are also influenced by contactwith other metals (due to galvanic corrosion). The code classifies the generalenvironment in which steel structures are exposed into five levels of severity asshown in Table 15.3.
15.8 Design of Steel StructuresTable 15.3 Environmental exposure conditions as per IS: 800 Environmental classifications Exposure conditions Mild Surfaces normally protected against exposure to weather or aggressive conditions as in the interior of buildings, except when located in coastal areas Moderate Structural steel surfaces exposed to (a) condensation and rain (b) water continuously (c) non-aggressive soil/groundwater (d) coastal areas but in the interior of buildings Severe Structural steel surfaces exposed to (a) severe frequent rain (b) alternate wetting and drying (c) severe condensation (d) sea water (completely immersed) (e) saturated salt air in coastal areas Very severe Structural steel surfaces exposed to (a) sea water spray (b) corrosive fumes (c) aggressive subsoil or ground water Extreme Structural steel surfaces exposed to (a) tidal zones and splash zones in the sea (b) aggressive liquid or solid chemicals Figure 15.5 shows the corrosion map of Indiashowing zones of corrosion.This explains why the iron pillar installed near the Qutub Minar (see Fig. 15.6) isshowing almost zero corrosion, whereas the speed of corrosion of structures inchemical and industrial areas is very rapid and hence need special attention. Structural steel in a mild environment and in the interiors of shops, schools,residences, hospitals, airport terminals, hostels, etc., will not corrode noticeablyduring the expected 5060 years life of the structure. In these situations no protectivecoating is required and the painting is done for decorative and aesthetic purposesonly. Only when the steelwork is exposed to moisture conditions such as thoseexisting in kitchens, bathrooms, or swimming pools, they may require a protectivecoating and attention is needed in the detailing of structural work. Some industrialbuildings, dairies, laundries, breweries, etc. need protective coatings of sufficientthickness. Structures exposed to high humidity and corrosive atmosphere, such aschemical plants, steel bridges, structures near coastal areas, and offshore structures,need better surface preparation and sufficient thickness of paint coating.15.2 Corrosion-protection MethodsMany different methods have been used to protect steel against rust. The mostobvious approach is to apply a protective coating to steel, thereby sealing off its
Corrosion Protection of Steel Structures 15.9 Fig. 15.5 Corrosion map of Indiasurface from a corrosive environment. Painting, zinc coating, and coating withvarious oils are examples of this method which have long been practised. Morerecently, thermal spraying of other metals, organic paints, and lining with rubberor porcelain enamel/plastic film lamination have come into use as protective coatingsfor steel. Another approach to corrosion protection is the use of steel that is not readilysusceptible to rust. Adding certain elements to steel during its production can modifythe inherent properties of steel so that a protective film forms on its surface. Thisapproach has produced stainless steel, first developed in the 1910s, and atmospheric-corrosion-resistant steel, which appeared in the 1930s. Electric protection is usedwhere a high corrosion resistance is essential or for structures such as steel pilesthat cannot be repaired. A good corrosion-protection system must take into account not only theeffectiveness of protection but also the technical ease of fabrication, reliability,
15.10 Design of Steel StructuresFig. 15.6 Iron pillar near the Qutub Minar, constructed in the 4th century B.C. by King Chandragupta IImaintenance, and overall economy. Among these factors, maintenance oftenreceives too little attention at the time of construction. Maintenance and its impacton the overall economy are among the most important factors in corrosion protection.No matter how effective a corrosion-protection system might be at the start, itseffectiveness is reduced at a later date due to chemical or mechanical damage, orboth. Organic coatings age, sacrificial anodes for cathodic protection is consumed,and corrosion-resistant steels are not entirely immune to corrosion. Inspection andmaintenance are necessary at proper intervals, and they are usually the most difficultand costly part of corrosion protection. Considering, for example, the maintenance of an offshore marine structure,inspecting the coatings in the splash zone, removing damaged coats, conditioningthe steel surface, and applying new coats under open-sea conditions are not easy.This point should be considered from the beginning. It is important to note that nocoating is completely impermeable. It is also interesting to note that there is acorrelation between the cost of a particular protection system and the degree of
Corrosion Protection of Steel Structures 15.11protection offered by it. Hence the selection of a particular system is largely basedon economics. The effectiveness of many corrosion-protection systems is affected by the surfacepreparation of the steel. Hence we shall discuss the methods of surface preparationbriefly in the following section.15.2.1 Surface PreparationTable 15.4 gives the various factors and their percentage contribution to thedurability of paint coatings. It is seen that surface preparation is the most importantfactor that affects the durability of paint coats.Table 15.4 Effect of various factors on the durability of paint coatings Factors Contribution (%) Surface preparation 49.5 Number of coats 19.1 Quality of paint 4.9 Others 26.5The various surface preparation methods which are used to clean the surface freeof dirt, mill scale, and other impurities and improve the adhesion of paints include(IS: 1477-2000) the following. l Hand scraping by means of a wire brush (economical but removes only 30% of the rust and scale). l Mechanical cleaning using power-driven tools (fast and effective and cleans up to 55% of rust and scale). l Flame cleaning (effective in removing mill scale, using differential thermal expansion caused by oxy-acetylene flame). l Sand blasting/grit blasting/shot blasting: Sand blasting is the common method adopted for structural applications, though some states in India disallow this method citing environmental reasons. This method uses the abrasive action of sand/grit (using angular particles)/iron shots (using spherical particles), which are projected at a high speed on the steel surface, using compressed air or an impeller. l Solvent cleaning (cleaning with a petroleum solvent such as turpentine). l Trichloroetheline cleaning. l Alkaline cleaning. l Oil or water emulsion cleaning. l Steam cleaning (steam at high velocity and high temperature is projected at the surface of steel). l High pressure water washing (water under high pressure, usually 8.3 to 34 MPa, is used to clean the steel surface). l Chemical cleaning called pickling (steel is immersed in a bath having very light sulphuric/hydrochloric or phosphoric acid to remove the rust). This method is opted for when hot-dip galvanizing is used.
15.12 Design of Steel Structures The choice of the solvent in cleaning depends on the type of the surface. Afterthe solvent or alkali or acid cleaning, the surface must be cleaned to make it freefrom the cleaner. We will now discuss the various corrosion-protection methods (see alsoIS: 9172-1979).15.2.2 PaintingPaints basically consist of a pigment, a binder (or medium), and a solvent (orthinner). After the paint has been applied as a wet film, the solvent evaporatesleaving the binder and the pigment on the surface. The pigment comprises finesolid particles which give the paint film colour and hardness, and inhibit corrosionby impeding the chemical or electrical processes. The binder is a resin or oil whichbinds the pigment particles together and provides a tough, flexible adhesive film.The solvent reduces the viscosity of the binder to allow even application. Thecharacteristics of common types of paints are given in Table 15.5, which can beused as a rough guide.Table 15.5 Main generic types of paint and their properties (Dowling et al. 1988)Paint type Cost Tolerance of Chemical Solvent Overcoat- Comments poor surface resistance resistance2 ability preparation1 after ageing3Bituminous Low Good Moderate Poor Good, with Limited to black coating of and dark colours, some type thermoplasticOil based Low Good Poor Poor GoodAlkyd, Low/ Moderate Poor Poor/ Good Good decorativeepoxyes- medium moderate propertiester, etc.Chlorina- Medium Poor Good Poor Good High-build filmsted rubber remain soft and are susceptible toVinyl High Poor Good Poor Good sticking during transportEpoxy Medium/ Very poor Very good Good Poor Susceptible to high chalking in UV lightUrethane High Very poor Very good Good Poor Better decorative properties than epoxiesInorganic High Very poor Moderate Good Moderate May requiresilicate special surface preparation1 Tolerance of poor surface: types rated poor or very poor should only be used on blast- cleaned surfaces.2 Solvent resistance: types rated poor or very poor should not generally be overcoated with any other type.3 Overcoating after ageing: types rated poor or very poor require suitable preparation of the aged surface if it is to be overcoated after an extended period.
Corrosion Protection of Steel Structures 15.13Specifying paint coating system must take into account the following: l Service life of the coating l Ease of painting l Place of coating in the total sequence of fabrication and erection steps l Severity of exposure to corrosion of various members l Ease of repairing l Maintenance cost Methods of painting include brush painting, spray painting, and airless spraypainting (IS 1477 : 2000, Part II). It has been estimated that the initial painting costof steel bridges is around 10% of the total construction cost. Repainting is a verysignificant item in the maintenance cost during the total life of a steel bridge. If thebridge is repainted 10 times (every five years during a total life span of 50 years),the repainting cost will be equal to the construction cost of the bridgeor possiblyeven greater! The application of paint can effectively prevent corrosion in two ways: by sealingoff the steel surface from the corrosive environment, or by the chemical action ofthe corrosioninhibiting pigment contained in the paint. The sealing properties of paints are due to the vehicle used. With the developmentof plastics, vehicles are now available in a great variety, from the solvent and watertypes to the chemical-reaction type and the powder type. Alkyd resin, melamineresin, urethane and other resins, phthalic resin, epoxy resin, chlorinated rubber,and other vehicles have been developed in rapid succession (see Table 15.5). Epoxypaints have found a particularly wide use in the corrosion protection of bridgesand ships because of their outstanding durability, mechanical strength, and resistanceto oil and chemicals. They also adhere well to the surface and can be applied inheavy coats. All paints may be subject to degradation by chemicals and by the UVradiation in the sunlight. They are also permeable to moisture and oxygen to someextent. Increasing the thickness of a paint coating increases the life of the structure. High-performance anti-corrosion paints in which the vehicle is blended withzinc, micaceous iron oxide, and other highly corrosionresistant pigments arealso widely used. Guidelines for a range of corrosion-protection systems forstructural frameworks for different environmental conditions as given in SteelConstruction Guide Book (The Kozai Club 1983) and ECCS Technical notes (1998)are shown in Table 15.6. The types of paint, their thickness in micrometers, andtheir frequency as recommended by the code for different environmental conditionsare given in Table 15.7. One coat of red oxide is normally applied before the material leaves thefabrication shop and another coat of it is applied immediately after erection at siteto prevent corrosion. A zinc- or aluminium-based primary coat is applied first,which serves as the foundation to the subsequent finishing coats. Some paints aretoxic in nature and hence some precautions have to be taken while applying them;some of these paints should not be sprayed/applied in confined spaces or used onmaterials that will be subsequently welded or flame cut. The film thickness of asingle coat of paint is about 0.035 mm for oil paint, about 0.025 mm for mostsynthetic resin paints, and about 0.015 mm for vinyl resin paint.
15.14 Design of Steel StructuresTable 15.6 Paint coating systems Coating system General coating system Heavy-duty coating system Corrosivity Mild Intermediate Severe Surface Blasting Blasting Blasting Blasting Blasting preparation of the steel section Shop primer Red lead/ Red lead/ Zinc chromate/ Inorganic Inorganic Red oxide Red oxide Zinc-rich Zinc-rich Zinc-rich primer primer Primer/ Lead- Lead- Chlorinated High-build High-build Undercoat pigmented pigmented rubber zinc-rich zinc-rich paint (1st coat) primer primer paint (mist-coat)1 Primer/ Lead- Lead- Chlorinated High-build High-build Undercoat pigmented pigmented rubber epoxy epoxy (2nd coat) primer primer Primer/ High-build High-build Undercoat epoxy epoxy (3rd coat) Intermediate Long-oil Phenol/ Chlorinated Polyurethane Epoxy coat phthalic MIO rubber Finish coat Long-oil Chlorinated Chlorinated Polyurethane Fluorinated phthalic rubber rubber resin Total coating 130 190 155 255 250 thickness (mm)1 Not included in the coating thickness.Source: ECCS, Technical Notes 90 and 88, 1998Table 15.7 Corrosion-protection treatment in external environment as per IS: 800 Shop-applied treatmentsCoatingSystem 1 2 3 4 5 6Surface Blast clean Blast clean Blast clean Blast clean Grit blast Blast cleanpreparationPrefabrica- Zinc phos- 2 pack zinc- 2 pack zinc- Ethyl zinction primer phate epoxy, rich epoxy, rich epoxy, silicate, 20 mm 20 mm 20 mm 20 mmPost fabrica- High-build 2 pack zinc- Hot-dip 2 pack zinc- Sprayed zinc Ethyl zinction primer zinc phos- rich epoxy, galvanize, rich epoxy, or sprayed silicate, phate modi- 20 mm 85 mm 25 mm aluminium 60 mm fied alkyd, 60 mmIntermedi- High-build 2 pack epoxy Sealer Chlorinatedate coat zinc phos- micaceous rubber phate, 25 mm iron oxide alkyd, 35 mmTop coat 2 pack epoxy Sealer micaceous iron oxide, 85 mm (contd )
Corrosion Protection of Steel Structures 15.15(contd ) Site-applied treatments1. Surface As As No site As No site As preparation necessary necessary treatment necessary treatment necessary2. Primer Touch in Touch in Touch in3. Intermedi- Modified Touch in High-build ate coat alkyd micaceous micaceous iron oxide, iron oxide, chlorinated 50 mm rubber, 75 mm4. Top coat High-build Modified High-build High-build alkyd finish, alkyd chlorinated micaceous 60 mm micaceous rubber iron oxide, iron oxide, chlorinated 50 mm rubber, 75 mm Expected life in yearsNormal 12 18 20 ±20 ±20 20+inlandPolluted 10 15 12 ±18 ±1520 20+inland1Normal 10 12 20 ±20 ±20 20+coastalPolluted 8 10 10 ±15 ±1520 20+coastal1For a desired life of 12 years in a polluted inland environment, coating system 3 to be selectedand so on. Paint should be applied in dry weather and attemperatures between +0.5°C and +50°C. Thetotal thickness of paint on a steel surface (primerplus finishing coats) should be as given below.For interior unclad steelwork(with ordinary humidity conditions) 130 mmIn industrial atmosphere 160 mmIn aggressive atmosphere 220 mmIn marine atmosphere 260 mm The 300-m-high Eiffel tower in Paris (see Fig.15.7) required 7300 tons of steel for itsconstruction. The tower still looks much as itwas on its completion in 1889, thanks to theproper painting at regular intervals for corrosionprotection. Fig. 15.7 Eiffel tower
15.16 Design of Steel Structures15.2.3 Lining and CoatingLinings are used to protect the internal surfaces of tanks and pipes in chemicalplants from corrosion. Coating in general protects the external surfaces of pipelines,plant piping, bridge cables, foundation piles, and structures. Depending on thesurface to be protected and the corrosive nature of the material contacting thesurface, appropriate lining and coating materials are chosen from among rubber,enamel, glass, concrete, and other inorganic or resin materials. One method of lining is to bond to the surface a lining material of film, sheet, ortape form. A paste-like lining material is applied to the surface with a trowel.Lining material in the powder form is either flame-sprayed or electro-staticallysprayed onto the surface. The method of application is determined by the size andshape of the structure to be lined. In many cases, the line pipe is mill-coated and lined. Lining of joints can beprovided at the construction site with ease, since lining materials are available inso many forms, such as film, tape, sheet, and tube. For offshore structures intended for service in the splash zone, which is mostcorrosive, various combinations of concrete coating, high-build type resin coating,and other methods are selected to suit the specified conditions of the installationsite.15.2.4 Hot-dip Galvanizing and Zinc Flame SprayingIn hot-dip galvanizing the structural members are immersed in a molten bath ofcoating metal at a temperature of about 450°C. This method is employed for suchmetallic coatings as zinc, aluminium, and tin which melt at lower temperaturesthan does iron (IS 4759 : 1996). Hot-dip aluminizing is only used for light sheetmaterial for high-temperature use (e.g., motor car exhausts). Lead also is coatedonto steel sheets in this manner, with the addition of small amounts of tin. The itemto be galvanized is first degreased and cleaned by pickling to enhance the adhesionproperties. In general, hot-dip galvanizing provides a relatively heavy coating(minimum 86 µm thickness or 610 g/m2) with high efficiency. One drawback isthat the size of the structural member that can be galvanized is restricted by thesize of the plating tank. Another drawback is the need for a large amount of energy.Because of the high temperature involved, it is important to ensure that any enclosedmembers, such as tubes, are vented to avoid the risk of explosion from vaporizationof the trapped moisture (Dowling et al. 1988). The zinc/iron alloy layer is harderthan the underlying steel and hence is resistant to the impact damage. In addition,this alloy layer gives perfect adhesion and total impermeability to moisture. Hot-dip galvanizing is employed for transmission towers, guardrails, bridges, etc.Galvanized members are often painted before use. For a given service environment,the useful life of a hot-dip galvanized structure is directly related to the thicknessof the zinc coating: the thicker the coating, the longer the useful life. Zinc flame spraying is generally used as a treatment for the base metal for coating.Unlike plating, this method puts no restriction on the size of the structure to be
Corrosion Protection of Steel Structures 15.17treated and can be used for on-site treatments. But it does have the drawback ofrequiring severe blasting of the surface to be treated. In industrial and marineatmospheres, aluminium coatings provide better corrosion protection than zinccoatings. A combination of metal-sprayed coatings and paintings achieve superiorprotection and is used for long-span bridges.15.2.5 Heavy-duty Coating SystemsThe paint system most commonly used for bridges presently is that consisting ofcorrosion-preventive oil paint/long-oil phthalic acid resin paint, about 130 mm thickcoating, which may be good only for three to four years in corrosive coastal areas.The epoxy resin zinc-rich paint/chlorinated rubber paint system is slightly better,but does not suffice the present need in severe environments. The use of thick, good quality paint coating systems with a repainting intervalof more than 10 years in severe atmospheres started some 25 years ago. Since thenthe systems have been improved and are now commonly used for major bridgeslocated at marine sites. They are called heavy-duty coating systems. Construction of large, long-span bridges has been active in Japan since 1960sbecause they have large economic and social effects. Most of them are locatedover straits or in bay areas. Representative examples are those of the Honshu-Shikoku bridge project that links the mainland (Honshu) with the south-westernisland of Shikoku with three routes that incorporate 17 bridges, the longest one(Akashi Kaikyo bridge) having a centre span of 1990 m (completed in 1998). Thedurability of paint coating systems is of critical importance for such large, long-span bridges because of the high corrosivity owing to the environmental factorsand the difficult accessibility for repainting. Based on an extensive study carriedout over 20 years, a paint system consisting of high-build zinc-rich paint, high-build epoxy (two coats) and polyurethane (two coats), and having a thickness of250 mm was specified for the first painting (1978) of this project. A system withhigh-build zinc-rich paint/high-build epoxy (two coats)/epoxy/fluorinated resinsystem, and having a thickness of 250 mm is also specified as per Matsushima(1997) (see Fig. 15.8). Fig. 15.8 Different layers of heavy-duty coating system The prime coat of zinc-rich paint is pigmented with a high concentration of zincdust, which, in contact with the steel surface, cathodically protects the latter in thesame manner as galvanized coating. Zinc metal spraying is sometimes specified
15.18 Design of Steel Structuresinstead of zinc-rich paints. The intermediate coats, such as epoxy resin, functionas a primer or protecting barrier, preventing intrusions of water, oxygen, anddetrimental ions. Otherwise the prime coats would deteriorate too soon due to therapid consumption of the zinc they contain. The intermediate coats also functionas a layer to secure good adhesions of the primer and the finish coat. The finishcoats, such as urethane, have good weathering resistance and protect the coatsunderneath from the detrimental action of sunshine (ultraviolet light) and water.More recent systems specify fluorinated resins as the finish coat for a longer servicelife. A typical fabrication procedure for heavy-duty coating systems includes shotblasting of the steel plates followed by an immediate application of a shop primer,fabrication of steel plates into blocks, shot-blasting of the blocks, and applicationof high-build zinc-rich primer. The shop primer provides temporary protectionduring the fabrication of the blocks. To ensure good adhesion between coats, eachovercoat must be applied within a certain time limit10 days to 6 months,depending on the type of paintafter complete curing of the previous coat, whichmay require one to two days. The surface of the previous coat must be cleanfreeof dirt and chlorides (less than 50 mg/m2). Most major bridges in marine areas are painted as per the above specificationsfor sections exposed to a severe environment. For example, Rainbow Bridge (centrespan 570 m, total length 798 m) completed in 1993 to link the Tokyo teleport townin Tokyo bay within the heart of Tokyo is coated with a high-build zinc-rich/high-build epoxy/epoxyMIO/fluorinated resin (two coats) system, 240 mm thick. In general, such heavy-duty corrosion-protection methods are more economicalthan the use of corrosion-resistant metals. In addition, heavy-duty methods spellcomparative ease of maintenance. Because of these advantages, heavy-duty methodsare adopted for an increasing number of structures.15.2.6 Cathodic ProtectionAs discussed earlier, when moisture is present, a steel surface behaves somewhatlike a batteryanode and cathode exist on the steel surface. This creates voltagedifferences that cause tiny currents to flow from anode to cathode and the circuit iscompleted through the moisture on the metal surface. The electrochemical reactionbetween iron and oxygen then results in the corrosion of the steel surface. In cathodicprotection, the flow of current is reversed, making the whole steel surface a cathode.This can be achieved in two ways: the impressed current method and the galvanicanode method (Kozai Club 1983).Impressed current method In this approach, shown in Fig. 15.9, a low-voltagedirect current is applied to the steel structure from a rectifier. The positive terminalof the rectifier is connected to an electrode (the anode) installed underwater orunderground, and the negative terminal is connected to the steel structure to beprotected.
Corrosion Protection of Steel Structures 15.19 Fig. 15.9 Impressed current method The electric current density can be controlled according to the rate of corrosion.Also, electrodes do not need frequent replacement. However, periodic inspectionand operating electric power are needed. The impressed current method is thuswell suited to large piers that require semi-permanent protection.Galvanic anode method If the steel structure is connected to electrodes made ofmetals that are lower in electric potential than iron, such as zinc, aluminium,magnesium or their alloys, a galvanic cell is formed in which the steel structureitself becomes the cathode. Thus the structure is protected while the anode getsgradually corroded. This approach is shown in Fig. 15.10. This method is simplerthan the impressed current method and involves a lower initial cost and requiresvery little maintenance. Fig. 15.10 Galvanic anode method15.3 Atmospheric-Corrosion-Resistant SteelsIn this section we will discuss two types of steels, viz., weathering steel and stainlesssteel, which are increasingly being employed in important structures. These steelsare produced by changing the chemical composition of mild steel and are consideredas corrosion resistant.
15.20 Design of Steel Structures15.3.1 Weathering SteelsThe corrosion resistance of steel may be improved by adding copper as an alloyelement. However, copper-alloyed carbon steel is very expensive and hence notused extensively. Stainless steels are high-alloyed steels and are discussed in thefollowing section. Atmospheric-corrosion-resistant steels are high-strength low-alloy steels that typically contain a combination of alloying elements such as copper,phosphorus, chromium, and nickel in small amounts (up to 3%). Originallydeveloped by United States Steel Corporation, these steels are called weatheringsteels and popularly known as Cor-Ten (Salmon & Johnson 1996). Cor-Ten matcheswith WR-Fe 480A of IS: 11587-1986. A comparison of the chemical compositionof weathering steel with other steels is given in Table 15.8. The reason for its lowsusceptibility to rusting is the same as that for stainless steel, since the base metalis protected against the corrosive environment by an oxide film, which is formedon its surface in the initial years of use. However, the mechanism by which thestable rust layer forms has not yet been fully studied. Generally, the formation of astable rust layer requires repeated cycles of wetting by rain and drying by sunshineand wind. Rust is produced on steel by the oxidizing reaction of iron. But theprotective film is formed in a different manner from that of stainless steel. In theearly stage of exposure, weathering steel begins to rust in the same way as ordinarycarbon steel. But later, after being subjected to repeated cycles of drying and wettingin the air, the initial layer of red rust transforms itself into a dark brown film whereverit contacts the steel surface. Within a few years, it becomes a stabilized, extremelyfine-textured rust film [which has the composition FeOOH (FeO3H2O)] that coversthe entire surface (Matsushima 1997). This film effectively prevents water andoxygen from reaching the steel beneath and thus halts the corrosion reaction almostentirely. Further rusting is thereby prevented. An added advantage is that sulphuricacid in the atmosphere, which stimulates the corrosion of ordinary steels, actuallypromotes the formation of the stable protective film in atmospheric-corrosion-resistant steels. A comparison of the reduction in the thickness for various steels isgiven in Fig. 15.11. The reduction in the thickness in 50 years would be less than0.3 mm in many atmospheres.Table 15.8 Comparison of chemical composition of various types of steel Type of steel Chemical composition (%) C Si Mn P S Cu Ni CrCarbon steel 0.16 0.009 0.57 0.010 0.010 0.11 0.025 0.036Copper-containing steel 0.13 0.152 0.55 0.071 0.011 0.39 0.025 0.035Atmospheric-corrosion-resistant steel (Type 1)1 0.11 0.467 0.30 0.119 0.021 0.39 0.410 0.640Atmospheric-corrosion-resistant steel (Type 2)1 0.10 0.458 0.37 0.103 0.021 0.29 0.280 0.7601Mo, Nb, Ti, V, and Zr are also added (0.15% maximum in total)
Corrosion Protection of Steel Structures 15.21Fig. 15.11 Comparison of weather resistance of steels (Steel Today and Tomorrow 1989) First introduced in 1958 in Illinois, USA, corrosion-resistant steels have alreadyfound application in buildings, bridges, and storage tanks, and their use continuesto grow. Because of their superior resistance to atmospheric corrosion, they arepainted (paint life is far longer than that of carbon steel) or coated with accelerantsthat hasten the formation of the protective film. The extra cost of such steel overordinary mild steel is about 20% and its use is amply justified in view of the heavycost of repeated painting. Though it was first produced in Japan in the 1960s, itwas used in bridges only during 1970s. Now about 20% of the steel bridges inJapan use weathering steel, accounting for about 50,000 tons of weathering steelused annually. Recently, Balasubramanian and his associates at the Indian Institute of Techno-logy, Kanpur, have developed a novel phosphorus-containing iron which would becorrosion resistant, ductile, and long lasting (Times of India 2005).Limitations of weathering steels Weathering steels perform properly when theconcentration of chlorides in the atmosphere or the accumulation of sulphuric acidfrom burned fuels is not excessive, and when water pools after rainfall do notremain for a long time. Significant amounts of deposited chlorides and continuouswet conditions hinder the formation of the protective rust film (Khanna 1999). The safe limit of the chloride concentration in the atmosphere is about 0.05 mgof NaCl/m2/day as determined by the wet-gauge method. Most sites 1 to 5 km orfurther from the sea coast or polluted industrial area satisfy this criterion, althoughin some areas where there is a strong prevailing wind from the sea, the criticaldistance inland from the sea coast may reach a maximum of 20 km. Also, weatheringsteels have no advantage over ordinary steels if buried in soil or totally immersedin water. In areas where a prolonged contact with water is unavoidable, such as theinterior of box girders, weathering steels need to be painted. It may take several years for the protective rust films to develop fully. It isnecessary to clean the steel surface for more uniform and smoother formation ofthe protective rust films. During the initial period, the corrosion rate is higher thanthat in the subsequent, well-protected period of service, and the run-off of rainwatermay colour the neighbouring concrete brown. Also, particles or flakes of rust mayspall off during this period.
15.22 Design of Steel Structures The fabrication and erection of weathering steel require care. Scale and disco-louration from welding should be removed and unsightly gouges, scratches anddents should be avoided (Khanna 1999).15.3.2 Stainless SteelsIn terms of chemical composition, stainless steels are broadly classified into high-Cr stainless steels, which contain chromium, and Ni-Cr stainless steels, whichcontain both chromium and nickel (Nagoya 1998; Subramanian & Sampath 2002).Representative grades are 13% Cr stainless, 18% Cr stainless, and 18% Cr and 8%Ni stainless steels. The general concept behind stainless steel is that a stabilized passive chromium-rich oxide film (3 mm thick) forms on its surface, preventing further penetration bythe corrosive atmosphere. The forming of such a film on the steel surface is calledpassivation. When chromium is added to steel in amounts of 11%13% or more,the fine textured passive film that forms provides significant resistance againstrusting (see Fig. 15.12). This film is ultra-thin, of the order of 1030Å. Its composi-tion can be expressed as Cr2O3NH2O. Unlike steel, which has a crystalline structure,the oxide film is amorphous, like glass, and is thought to be a uniform and chemicallystable film. When it is marred, the film is immediately repaired by the action of Crions. But once the protective film has been destroyed under certain circumstancesFig. 15.12 Graph showing the relation between chromium content and corrosion (Nagoya 1998)
Corrosion Protection of Steel Structures 15.23(especially in coastal areas, where sea salt particles are deposited on the surface,damage this passive film, and eventually lead to small pitting), stainless steelsbecome susceptible to rusting. Thus it cannot be said that stainless steels neverrust. Nonetheless, they are highly resistant to rusting. Steel manufacturers haverecently stepped up their development efforts in this field, with emphasis on newtechnology that speeds up the formation of the passive film. The addition of suchelements as molybdenum, copper, titanium, and niobium, for example, makes thefilm form more quickly. Tests conducted in Japan show that the maximum depth ofpitting corrosion is only 0.2 mm even after 40 years for type SUS 304 steel (producedin Japan). Designability is another advantage offered by the use of stainless steel.A variety of stainless steel sheets having attractive colours and patterns have beenintroduced. Figure 15.13 shows the Osaka Dome in Japan, which is covered withstainless steel sheets, and Fig. 1.40 shows a double-layer grid in India using stainlesssteel tubular members. The recent developments in the field of stainless steel include (Nagoya 1998;Subramanian 2000) the following. 1. Superior weather-resistant stainless steel for use at waterfronts (ferritic steels SUS444 of 19% Cr-2% Mo type). The roof of the Japan Sea Base pavilion is of a new high-alloy steel (30 Cr-2 Mo type) having weather resistance comparable to that of titanium. Compared to SUS 304 (18% Cr-8% Ni steel), this stainless steel not only has a higher localized corrosion resistance in a chloride environment but also avoids stress corrosion cracking entirely in a hot water environment. 2. Metal coated stainless steels. In these either aluminium or zinc is coated onto the surface of stainless steel.Fig. 15.13 Osaka Dome built in Japan in 1997 (Courtesy: Steel Today and Tomorrow)
15.24 Design of Steel Structures3. Pre-painted stainless steel in which silicon polyesters and acrylics are painted on the surface of stainless steel. Recently fluorocarbon resins have also been introduced. Various transparent painting systems, which do not destroy the decorativeness of stainless steel, have also been developed recently.More details about stainless steel are given in Section 22.214.171.124 Corrosion AllowanceThe concept of protection by corrosion allowance can be applied to projectsinvolving steel piles, steel sheet piles, offshore structures, and other steel structuresplaced underground or underwater. In the design of a steel pipe pile, for example, a wall thickness is calculated foreach section of the pile that ensures safety with respect to compression, tension,bending, shear, and other stresses which may arise in service. Then an extra wallthickness is added, equal to the expected loss in the thickness due to corrosionduring the intended service life of the pile. When the corrosion allowance approachis used, a clear knowledge of the rate of corrosion of underground and sub-seasteel installations is necessary. In Japan it has been found that the rate of corrosionaveraged a mere 0.024 mm per year. This shows that a pile, if given a corrosionallowance of 2 mm in the wall thickness, has a life expectancy of 80 years.15.5 Detailing to Reduce CorrosionIt is also important that the detailing of steel structures should be done in a waythat enhances durability. Some of the points to be considered are (see Fig. 15.14)as follows. 1. The detailing should avoid water or dirt entrapment or accumulation in corrosion points, such as sharp and re-entrant corners, cavities, welded rough surfaces, to avoid corrosion due to accumulation of dust and moisture. 2. Discontinuous weld points, spot welds, and tubular edge welds are also trouble spots of corrosion. All such points should be cleaned and filled or smoothened with tar-paint to protect from corrosion. 3. Detailing should provide suitable drainage breaks or holes wherever possible so that water does not accumulate. 4. Detailing should encourage free air movement such that the surfaces are dried rapidly. 5. Detailing should avoid crevices as far as possible. 6. Suitable access to all the components of the steel structure (especially the joints in a bridge) should be provided for periodic inspection and maintenance. 7. Detailing should avoid contact with different materials to prevent galvanic corrosion. 8. When friction grip bolts are used, protective treatment should not be applied to the faying surfaces.
Corrosion Protection of Steel Structures 15.25 Fig. 15.14 Detailing to avoid water entrapment (ECCS 1998)15.6 Encasing in ConcreteTraditionally steel members are encased in concrete to prevent corrosion [seeFig. 1.46(a) and (c)]. Encasing steel in concrete provides an alkaline environmentdue to the hydration of cement (the pH value of concrete is of the order of12.513.5). This results in the formation of a protective film of iron oxide on thesurface of steel components. This passive protection is broken when the pH valueof the regions adjoining the steel falls below about 9. This can occur due to thefollowing: l Water diffusion through the pores of concrete (carrying with it SO 2 and CO2 gases from the air in the form of weak acids) l Carbonation (reaction of carbon dioxide in the atmosphere with the alkalis in the cement paste) l Ingress of soluble chloridesthe extent of penetration depends on the permeability and thickness of concrete
15.26 Design of Steel StructuresThe resulting corrosion of steel and the increase in pressure result in spalling ofconcrete. It has to be noted that the members that are encased in concrete shouldneither be painted nor oiled. Encasing steel members in concrete increases thedead load of the structure and results in increased foundation costs. Moreover, thesteel members are not visible for inspection or repair; hence concrete encasing isnot suggested now-a-days as a corrosion-protection method.SummaryThe durability of structures is given more emphasis in recent times. Durability andcorrosion are considered as serviceability limit states criteria. A durable steelstructure may be defined as the one that performs satisfactorily the intendedfunction(s) in the working environment under the anticipated exposure condition(s)during its service life, without any deterioration of the cross-sectional area andloss of strength due to corrosion. Corrosion of steel is an electrochemical process which will not occur unlesswater and oxygen are both present on the steel surface. There are several types ofcorrosion. The results of surveys conducted in several countries show that theannual loss due to corrosion amounts to several million dollars. However, withsuitable corrosion control methods, the rate of corrosion can be made vary slow orpractically nil. The rate of corrosion depends mainly on the degree of atmospheric pollutionand the duration of wetness of the steel surface. Local corrosion rates are alsoinfluenced by contact with other metals. IS: 800 classifies environment into fivedifferent categories: mild, moderate, severe, very severe, and extreme. Each classof environment requires a different kind of corrosion protection. It is seen that thecorrosion rate inside buildings is insignificant, since the steel members inside thebuildings do not come into contact with moisture. The most common type of corrosion protection is to apply a protective coatingto steel, thereby sealing off its surface from a corrosive environment. However, theperformance of such coatings depends largely on the correct surface preparationbefore coating. The blast cleaning process, in which abrasive particles are projectedat a high speed onto the steel surface, produces a clean and rough surface thatimproves the adhesion of coatings. Shot blasting is preferred for most paint coatings,whereas grid blasting is used for sprayed metal coatings. Chemical cleaning maybe opted for when hot-dip galvanizing is used. Many generic types of paints are available and guidelines to use these paints indifferent environments are given. While specifying paint coatings, one should takeinto account the severity of exposure, ease of painting, sequence of fabrication anderection, ease of repairing, and maintenance cost. Linings are used to protect theinternal surfaces of tanks and pipes in chemical plants and external surfaces ofpipes, bridge cables, and foundation piles. Hot-dip galvanizing, in which the steel members are dipped into a bath of moltenzinc or aluminium kept at about 450°C, is the cheapest and most common method
Corrosion Protection of Steel Structures 15.27of metal coating. Metal spraying uses a special spray gun to throw molten zinc oraluminium coating onto a clean, grit-blasted surface. No alloying takes place inmetal spraying. Metal spraying may be provided with a sealing treatment to givemaximum corrosion resistance. However, the cost of sprayed coatings is high dueto the required surface preparation. Heavy-duty coating systems with thicknesses up to 250 mm have been used insteel bridges located in severe environments. Cathodic protection in the form ofthe impressed current method and the galvanic anode method is used in structureswhere a high corrosion resistance is essential or in structures that cannot be easilyrepaired. Low-alloy steels with alloying elements such as copper, phosphorus,chromium and nickel, called weathering steels and stainless steels, containingchromium and nickel have been used extensively in the recent past. Though theinitial cost of these steels is high, the life cycle cost analysis has proved them to beeconomical in the long run. Though concrete encasement provides an alkalineenvironment that protects the steel member, it increases the dead weight and henceis not used extensively as a corrosion protection system. Since longer periods of wetness result in greater corrosion, it is important todesign and detail the structures in such a way that they shed the water rather thanretain it. Wherever necessary, drainage holes of appropriate sizes and at appropriatelocations should be provided to ensure that all the water is drained from the memberand there is a free flow of air to promote rapid drying. More details about the corrosion protection of steel structures may be found inPimple et al. (2002), Samanta (2003a), Chaudhari and Samanta (2003), and Samanta(2003b). Review Questions 1. Explain the process of corrosion. 2. What are the three things that must be eliminated in order to prevent corrosion? 3. Does rust formation prevent corrosion? 4. What are the different types of corrosion? 5. Write short notes on the following: a. Uniform corrosion b. Pitting corrosion c. Crevice corrosion d. Galvanic corrosion e. Stress corrosion f. Corrosion fatigue g. Intergranular corrosion 6. What is hydrogen embrittlement? 7. The thickness of the rust layer will be a. Equal to the thickness lost in the original steel b. Less than the thickness lost in the original steel c. Double the thickness lost in the original steel d. Four times the thickness lost in the original steel
15.28 Design of Steel Structures 8. What are the factors that influence the rate of corrosion? 9. Match the following: a. Severe environment a. interior of building b. Extreme environment b. structures under water c. Moderate environment c. structures in coastal area d. Mild environment d. structure in chemical factory10. What are the factors to be considered while selecting a corrosion-protection system?11. Match the following: a. Structures in remote areas a. heavy-duty coating system b. Members inside building b. cathodic protection c. Industrial building c. oil-based painting d. Bridges d. chlorinated rubber painting e. Steel piles e. hot-dip galvanizing12. List the various corrosion-protection methods.13. What are the different surface preparation methods?14. What type of surface preparation is used for hot-dip galvanizing?15. What is the use of surface preparation?16. What are the factors to be considered while specifying a paint coating system?17. What are the main components of a paint coating system?18. List some of the available types of paints.19. What is the thickness of paint to be applied for interior members in mild environment and members in industrial environment?20. Where are linings used and what are the materials used for lining?21. Write short notes on the following: a. Hot-dip galvanizing b. Zinc flame spraying c. Heavy-duty coating system d. Cathodic protection e. Weathering steel f. Stainless steel22. What is the difference between weathering steel and stainless steel?23. What are the limitations of weathering steel?24. What is meant by corrosion allowance?25. Why concrete encasing is not preferred as a corrosion-protection method?26. What are the points to be considered while designing and detailing steel structures in order to reduce corrosion and enhance durability?